the effectiveness of fluoride ( f ) varnishes has been well established in caries prevention studies involving permanent teeth11.clinical studies have demonstrated a decline of caries incidence from 18 up to 70%15 .
therefore , the use of f varnishes has been recommended for children at high or moderate risk to develop dental caries21 .
moreover , it is the only product recommended for children up to 6 years of age who have special health care needs17 .
recently , the decrease in s. mutans counts after f varnish application has also been reported12 .
they adhere to the teeth and enhance f release to the enamel surface , dental plaque and saliva .
this adhesion also enables the application in small amounts , decreasing the risk of f over - ingestion23 .
a previous work from our research group showed differences on anticariogenic action and calcium fluoride ( caf2 ) formation in seven marketed varnishes available in brazil as a result of variations on physical properties of f varnishes14 .
physical properties can influence the activity of f varnishes on enamel surface . considering that the contact time between the fluoride product and the enamel surface is very important to the efficacy of this preventive measure23
, the use of some materials could avoid f loss to saliva and , consequently , improve its anticariogenic effect .
the aim of this study was to evaluate the effect of an experimental coat on the anticariogenic action of fluoride varnishes .
two market varnishes were used : duraphat ( " dura " ; 5% naf , a. nattterman & cie . gmbh . , colony , germany ) and duofluorid xii ( " duo " ; 6%
the coat has the same composition as that of duofluorid xii ( dentscare ltda , joinville , sc , brazil ) but does not contain fluoride .
the coat was applied over the fluoride varnishes , as a second layer , and was also used in the placebo group ( negative control ) .
enamel blocks ( 4x4 mm ) were obtained from bovine incisors previously stored in a 2% formaldehyde solution at ph 7.0 for 30 days at room temperature24 .
the enamel surfaces were serially polished and the blocks were selected based on the surface microhardness ( smh ) ( 324.8 up to 357.0 khn ) and were randomized into five groups ( n=12 ) : a ) coat only ( " placebo " ; varnish without fluoride ) , b ) dura , c ) dura with the experimental coat ( dura + coat ) , d ) duo and e ) duo with the experimental coat ( duo + coat ) . the blocks were subjected to seven days of a ph - cycling model based on vieira , et al.24 .
initially , the enamel was treated with the varnishes and coat , if applicable , and placed in a demineralizing solution ( " de " : 2.0 mmol l calcium and phosphate in 75 mmol l acetate buffer , ph 4.7 ; 0.04 g f / ml , 2.2 ml / mm ) .
after 6 h , the varnishes were removed with a blade and acetone5 and the blocks were transferred to a remineralizing solution ( " re " : 1.5 mmol l calcium , 0.9 mmol l phosphate , 150 mmol l kcl in 0.1 mol l cacodylic buffer , ph 7.0 ; 0.05 mg f / ml , 1.1 ml / mm ) for 18 h. on the second day , both solutions were changed due to f release from the varnishes .
the 6 and the 7 day , the enamel blocks were kept in the remineralizing solution .
after ph cycling , aliquots of the solutions were mixed with tisab ii ( total ionic strength adjustment buffer ) at 1:1 tisab ii : sample ratio ( ph 5.2 ) and the amount of f in the solutions was analyzed , using an ion - selective electrode ( orion 96 - 09 ; orion research inc .
, beverly , ma , usa ) and a digital ion analyzer ( orion 720a ; orion research inc . ) , surface ( smh ) and cross - sectional ( csmh ) microhardness measurements were made on enamel surface as described before24 , except for the fact that the load used was 25 g. the % smhc was calculated .
the csmh values were converted to mineral content by volume , according to featherstone , et al.9 . the integrated mineral loss ( z ) after ph cycling was calculated1,18 .
the loosely - bound fluoride ( caf2 ) was analyzed to evaluate the amount of caf2 present after fluoride varnish application ( caf2 formed ) or to analyze the amount of caf2 that was still adsorbed to the enamel after ph - cycling ( caf2 retained ) . in order to assess
caf2 formed , 12 blocks from each group were treated as described above , but were subjected to only one 24 h cycle .
the enamel blocks were immersed in 0.5 ml koh 1mol l for 24 h under agitation .
fluoride measurement was performed with an ion - selective electrode orion 96 - 09 ( orion research inc . ) and an ion analyzer orion 720 a+ ( orion research inc . ) , calibrated with standards containing 0.0625 up to 2.0 g f / ml . the results were expressed as g f / cm .
the null hypothesis tested was that the use of the experimental coat does not improve the anticariogenic action of fluoride varnishes .
data from z , caf2 formed , caf2 retained and f present in solutions were not normal and had a non - homogeneous distribution .
thus , kruskal - wallis test was used at each data point . for % smhc ,
the difference between caf2 formed and caf2 retained was evaluated with the non - paired t test .
two market varnishes were used : duraphat ( " dura " ; 5% naf , a. nattterman & cie . gmbh . , colony , germany ) and duofluorid xii ( " duo " ; 6%
the coat has the same composition as that of duofluorid xii ( dentscare ltda , joinville , sc , brazil ) but does not contain fluoride .
the coat was applied over the fluoride varnishes , as a second layer , and was also used in the placebo group ( negative control ) .
enamel blocks ( 4x4 mm ) were obtained from bovine incisors previously stored in a 2% formaldehyde solution at ph 7.0 for 30 days at room temperature24 .
the enamel surfaces were serially polished and the blocks were selected based on the surface microhardness ( smh ) ( 324.8 up to 357.0 khn ) and were randomized into five groups ( n=12 ) : a ) coat only ( " placebo " ; varnish without fluoride ) , b ) dura , c ) dura with the experimental coat ( dura + coat ) , d ) duo and e ) duo with the experimental coat ( duo + coat ) .
the blocks were subjected to seven days of a ph - cycling model based on vieira , et al.24 .
initially , the enamel was treated with the varnishes and coat , if applicable , and placed in a demineralizing solution ( " de " : 2.0 mmol l calcium and phosphate in 75 mmol l acetate buffer , ph 4.7 ; 0.04 g f / ml , 2.2 ml / mm ) .
after 6 h , the varnishes were removed with a blade and acetone5 and the blocks were transferred to a remineralizing solution ( " re " : 1.5 mmol l calcium , 0.9 mmol l phosphate , 150 mmol l kcl in 0.1 mol l cacodylic buffer , ph 7.0 ; 0.05 mg f / ml , 1.1 ml / mm ) for 18 h. on the second day , both solutions were changed due to f release from the varnishes .
these solutions were kept until the 5 day . during the 6 and the 7 day ,
after ph cycling , aliquots of the solutions were mixed with tisab ii ( total ionic strength adjustment buffer ) at 1:1 tisab ii : sample ratio ( ph 5.2 ) and the amount of f in the solutions was analyzed , using an ion - selective electrode ( orion 96 - 09 ; orion research inc .
, beverly , ma , usa ) and a digital ion analyzer ( orion 720a ; orion research inc . ) ,
surface ( smh ) and cross - sectional ( csmh ) microhardness measurements were made on enamel surface as described before24 , except for the fact that the load used was 25 g. the % smhc was calculated .
the csmh values were converted to mineral content by volume , according to featherstone , et al.9 . the integrated mineral loss ( z ) after ph cycling was calculated1,18 .
the loosely - bound fluoride ( caf2 ) was analyzed to evaluate the amount of caf2 present after fluoride varnish application ( caf2 formed ) or to analyze the amount of caf2 that was still adsorbed to the enamel after ph - cycling ( caf2 retained ) . in order to assess
caf2 formed , 12 blocks from each group were treated as described above , but were subjected to only one 24 h cycle . the analysis of caf2 retained was done in the ph - cycled blocks .
the enamel blocks were immersed in 0.5 ml koh 1mol l for 24 h under agitation .
fluoride measurement was performed with an ion - selective electrode orion 96 - 09 ( orion research inc . ) and an ion analyzer orion 720 a+ ( orion research inc . ) , calibrated with standards containing 0.0625 up to 2.0 g f / ml . the results were expressed as g f / cm .
the null hypothesis tested was that the use of the experimental coat does not improve the anticariogenic action of fluoride varnishes .
data from z , caf2 formed , caf2 retained and f present in solutions were not normal and had a non - homogeneous distribution .
thus , kruskal - wallis test was used at each data point . for % smhc ,
the difference between caf2 formed and caf2 retained was evaluated with the non - paired t test .

 table 1 shows that the application of the coat was not able to improve either % smhc or z moreover , when comparing the varnishes , there were no differences on surface demineralization ( % smhc ) but the lesion depth ( z ) for the groups treated with duo was shallower when compared to the groups treated with dura ( table 1 ) .
different uppercase letters indicate statistically significant differences between caf2 formed or caf2 retained ( non paired t test , p<0.05 ) .
kruskal - wallis , p<0.05 in addition , the presence of the coat allowed greater formation of caf2-like material for duo+coat , but not for dura+coat , when compared to the respective commercial varnishes without the coat .
greater retention of caf2 was observed for both varnishes associated with the coat . for all treatment groups , except for placebo ,
f release to the solutions de1 , re1 and de2 was different in all treatment groups .
furthermore , the groups treated with duo showed higher amount of f in the ph - cycling solutions .
the presence of the coat decreased f release in de1 . on the other hand ,
after the coat was removed , the groups duo+coat and dura+coat presented the highest amount of f in the solutions re1 and de2 . in the last 2 days of ph - cycling , the groups duo and duo+coat showed higher amount of f in re2 when compared to dura or dura+coat , regardless of whether the coat was applied or not ( table 2 ) .
means followed by different letters indicate statistically significant difference between the groups ( kruskal - wallis , p<0.05 ) .
calcium fluoride is the main product formed after the application of a topical fluoride , especially with highly concentrated f products .
the amount of caf2 formed depends on the ph , the duration of exposure and the f concentration in the products19 , and it is very important for the efficacy of fluoride varnishes .
the fact that duofluorid xii has twice the f concentration of duraphat certainly contributed to the highest amounts of caf2-like material observed in duo and duo+coat groups , which is probably originated from the pure caf2 present in duofluorid xii. this may also explain the shallower the lesion depth ( z ) and the higher amount of f in all solutions analyzed for the groups duo and duo+coat when compared to dura and dura + coat .
another reason for these results is the fact that the synthetic resin base of duofluorid xii makes the varnish less viscous and dense , which leads to a higher ability to release f in their matrixes7,20 . analyzing the f released in the solutions and the caf2 in enamel , an overall f kinetics during the ph cycling
the f that was not released to the solutions during the first 6 h of ph - cycling ( when the coat was present ) contributed to the formation of caf2 .
when the varnishes were removed the groups that received the coat treatment showed a higher amount of f released in " re 1 " because more caf2 was formed on the enamel . with this observation , it may be assumed that caf2 was readily loss to the medium as soon as the coat was removed in spite of the higher amount of caf2 formed in the presence of the coat .
this event may have contributed to the lack of efficacy of the coat regarding % smhc and z .
this observation is also confirmed by the high release of f for the coat groups in " de 2 " .
still , the coat did not influence the amount of f released in the last two days of ph - cycling ( " re2 " ) .
attin , et al.2 found that f is leached away within the experimental period after a topical application of bifluorid 12 ( voco gmbh , cuxhaven , germany ) or duraphat. another interesting finding of the present study was that caf2 retained was higher than caf2 formed only in the placebo groups .
this can be attributed to the ph cycling model used in the present study , which had a high acid challenge .
the dental enamel becomes more reactive as enamel demineralization increases , which could have facilitated the deposition of f from the solutions , even if it was present at low concentrations .
moreover , the presence of the coat was not able to improve either % smhc or z possibly because the amount of caf2 was not high enough to induce a sensible change in enamel demineralization .
it is probably necessary very high differences of caf2 , such as that observed between duraphat and duofluorid to detect changes in lesion depth or even higher amounts to show changes in surface microhardness .
f varnish can be clinically applied to prevent proximal caries22 , enamel demineralization during orthodontic treatment8 , early childhood caries13 .
prevention of proximal caries by f varnishes showed better results compared to fluoride mouthrinsing and the cost - effectiveness ratio observed was 1.822 . due to the wide variety of clinical applications and the effectiveness of f varnishes ,
recently , two new f varnishes , including a bioerodible material , has been evaluated4,16 and showed good results .
it may be concluded that the application of the experimental coat reduced the amount of f released and increased the formation of caf2 , but it was not able to enhance the anticariogenic action of the f varnishes .
 objective : the time of contact between the product and enamel surface is important in ensuring the efficacy of fluoride varnishes . 
 thus , some alternatives could avoid fluoride loss to saliva and improve the anticariogenic action of the product . 
 this study evaluated the effect of an experimental coat on the anticariogenic action of fluoride varnishes.material and methods : enamel bovine blocks were selected by evaluating surface microhardness and randomized into five groups ( n=24 ) : placebo , duraphat , duraphat with coat , duofluorid and duofluorid with coat . 
 twelve blocks from each group were used to analyze calcium fluoride ( caf2 ) formed on enamel after treatment . 
 the other 12 blocks were subjected to ph cycling for 7 days . 
 the varnishes were kept on enamel for 6 h. next , the percentage change of surface microhardness ( % smhc ) and mineral loss ( z ) were calculated . 
 caf2 retained and fluoride present in the ph - cycled solutions were also measured.results:the use of the coat did not decrease % smhc and z , but all fluoride varnishes had better results when compared to the placebo ( anova and kruskal - wallis , respectively ) . 
 the values from caf2 formed were higher compared to the values of caf2 retained ( non - paired t test , p<0.05 ) . 
 there was a trend to decrease the amount of f in the solutions at the end of ph cycling ( kruskal - wallis , p<0.05).conclusions : although the experimental coat increased the formation of caf2 on the enamel surface , it did not significantly improve the anticariogenic action of fluoride varnishes . 
INTRODUCTION
MATERIALS AND METHODS
Experimental Groups
pH-cycling and Treatment with F varnishes
Microhardness Analysis
Calcium Fluoride (CaF
Statistical Analysis
RESULTS
DISCUSSION
CONCLUSION